244 D. S. RAWAL et al : A REPRODUCIBLE HIGH ETCH RATE ICP PROCESS FOR ETCHING OF VIA-HOLE GROUNDS IN…
A Reproducible High Etch Rate ICP Process for Etching
of Via-Hole Grounds in 200 µm Thick GaAs MMICs
D. S. Rawal, Vanita R. Agarwal, H. S. Sharma, B. K. Sehgal, and R. Muralidharan
Abstract—An inductively coupled plasma etching strongly desired to improve the wafer throughput and to
process to replace an existing slower rate reactive ion reduce the cycle time. Inductively Coupled Plasma (ICP)
etching process for 60 μm diameter via-holes using etching has been replacing conventional reactive ion
Cl2/BCl3 gases has been investigated. Process pressure etching (RIE) for GaAs backside via etching because of
and platen power were varied at a constant ICP coil several advantages. Throughput improvement utilizing signi-
power to reproduce the RIE etched 200 µm deep via ficantly faster etching rate have already been reported in
profile, at high etch rate. Desired etch profile was the literature [4,5]. Furthermore, the ICP tools provide
obtained at 40 mTorr pressure, 950 W coil power, better control of via size, repeatability and reproduce-
90W platen power with an etch rate ~ 4 μm/min and bility .
via etch yield >90% over a 3-inch wafer, using 24 μm The ICP tools produce significantly different via di-
thick photoresist mask. The etch uniformity and mension as compared to the conventional RIE tools, if
reproducibility obtained for the process were better the same size mask used, due to its nature of etching
than 4%. The metallized via-hole dc resistance measured process. Generally, ICP produces a vertical profile utili-
was ~ 0.5 Ω and via inductance value measured was zing low pressure and higher ion density process while
~ 83 pH. RIE produces a conical shape. The etch profile and
surface morphology of via-hole grounds is important not
Index Terms—GaAs, MMIC, via-hole, ICP, etching only for the inductance consideration but also for the
success of backside metallization. The smooth morpho-
logy of the etched sidewalls provides reliable and good
electrical contact with low resistance.
Etching is mainly carried out in chlorine/fluorine
The backside via-hole is one of the most critical elements
plasma. A number of gas combinations CCl2F2, CCl2F2/
for Monolithic Microwave Integrated Circuit (MMIC)
CCl4, SiCl4/Cl2, BCl3/Cl2/Ar, Cl2/Ar and Cl2/BCl3
technology. Electrically it provides a low inductance/resis-
have been utilized to fabricate via-holes . Each gas
tance contact to the common grounding plane and at the
combination has its advantages and disadvantages. CCl2F2
same time thermally serves as a heat dissipation path for
is attractive because of its excellent selectivity with
Metal Semiconductor Field Effect Transistors (MESFET)
respect to front-side metal (Ti/Pt/Au, Cr) and lack of
and High Electron Mobility Transistors (HEMT)[1-3].
corrosiveness and toxicity, but the etch rate is too low
Backside via etching is often a bottleneck of wafer
and severe polymer formation occurs on the etched area
production due to its crucial nature of very deep (100-
as well as on the chamber walls resulting in poor process
200 µm) through substrate etching, after front side
reproducibility. Cl2/BCl3 gas mixture with ICP process
processing is complete. Thus, an optimized process is
is being increasingly used for fabrication of via-holes at
high etch rates with excellent anisotropy and smooth
Manuscript received Aug. 11, 2008; revised Sep. 3, 2008. surface morphology.
Solid State Physics Laboratory, Delhi-110054, India
E-mail : firstname.lastname@example.org For the implementation of ICP backside via etching
JOURNAL OF SEMICONDUCTOR TECHNOLOGY AND SCIENCE, VOL.8, NO.3, SEPTEMBER, 2008 245
process into any existing RIE etching production line, it ICP system, one at a time. An oxygen plasma de-scum
is important to understand the impact of ICP process step prior to etching was utilized in order to remove any
parameters on via profile, etch rate, mask selectivity, residual photoresist in via-hole which would otherwise
sidewall morphology and produce same RIE via etch contribute to the roughness of the etched surface. Plasma
profile to avoid any changes in via model and circuit of etcher is inductively coupled through a coil at 13.56 MHz,
design. A slight change in via etch profile would lead to with independent energy control provided by 13.56 MHz
change in via inductance value of grounded source pad. RF biasing of the wafer platen. Helium gas is used to
This change in source inductance could affect the circuit help cool backside of the wafer. The substrate tempera-
performance for higher frequency application. In parti- ture was set at 20 °C for all test conditions. The etch
cular, the low noise amplifier (LNA) circuits where chemistry is a mixture of Cl2/BCl3 through mass flow
source impedance feedback is often used as a means to controlled process gas lines. The chamber was evacuated
achieve more stability may be more vulnerable to the to a base pressure of 9E-6 Torr, by a turbomoleculer
subtle unwanted source inductance changes due to the pump backed by a dry mechanical pump, before initiating
change of via dimension. Reproducing RIE etch profile the etch process. The etch gases mixture was introduced
with ICP process would enhance the throughput signify- through an annular region at the top of chamber lid. ICP
cantly without affecting the production using existing Process parameters like pressure and platen power were
designs. Otherwise, all the circuit designs will have to varied in a narrow window, at constant ICP coil power,
incorporate via dimensional changes and has to go to reproduce the RIE etched 200µm deep via profile at a
through expensive mask set fabrication step. relatively very high etch rate. The etch rate, etch depth,
Generally reported etch depths using ICP/RIE for via- etch profile and surface morphology of via-holes were
hole etching applications in MMIC are less than 200 µm determined by cleaving through the etched features and
using photoresist mask [5-8]. In this study, we are examining the sample under scanning electron micro-
reporting the etching of 60 µm diam. via-holes, up to a scope, model LEO-1430.
depth of 200 µm, in 3- inch GaAs wafer using positive
photoresist mask. III. RESULTS AND DISCUSSION
The aim of this study has been to replace the existing
via-hole RIE process using CCl2F2/CCl4 gases, with new Fig. 1 shows the targeted an-isotropic etch profile of a
reproducible ICP process using non-CFC gas chemistry 200 µm deep via-hole obtained with the RIE process at a
(Cl2/BCl3), for in-house MMICs production line without relatively slow etch rate ~ 1.3 µm/min. Via profile obtained
changing existing MMIC designs and mask sets. was conical in shape with 60±10 µm diameter opening
on front side and 180±10 µm diameter opening on
II. EXPERIMENTAL backside of wafer respectively. The details of this work
All test samples were 650 µm thick, 3- inch S.I. GaAs
wafers with front side pattern. These wafers were mounted
on 82 mm diameter sapphire carrier with wax, front side
facing down and thinned down to 200±10 µm by standard
lapping and polishing method. The substrate thickness
was kept 200 µm considering factors like handling of
fragile wafers and electrical losses in MMIC micro-strip
interconnects on the front side. Wafers were then coated
with 24 µm thick positive photo resist AZ 4620 and
exposed to define via-holes with 60 µm diameter. The
patterned photoresist was post baked at 120 °C for 30
minutes to introduce a sloped photoresist profile with Fig. 1. 200 µm deep via etch profile obtained using standard
improved adhesion. All the wafers were etched in standard RIE process.
246 D. S. RAWAL et al : A REPRODUCIBLE HIGH ETCH RATE ICP PROCESS FOR ETCHING OF VIA-HOLE GROUNDS IN…
are already published elsewhere .
All the ICP experiments were carried out at near maxi-
mum available coil power and Cl2/BCl3 flow rate ratio
of 4:3 to have high plasma density  and increased
concentration of reactive Cl species that resulted in high
etch rates with better etch surface morphology. Higher
than 4:3 flow rate ratio increased the etch rate but at the
cost of surface morphology, whereas lower flow rate
ratio decreased the etch rate significantly. Fig. 2 shows
the etch rate variation with elapsed etch time for ICP
process at 950 W coil power, 30 mTorr pressure and 65
W platen power. It clearly shows that the average etch
Fig. 3. ICP etched via profile obtained after 45 minutes of
rate is decreased with etch time, from 7 µm/min for 10 etching at 30mTorr.
minute of etching to 3.9 µm/min for 45 minutes of
etching on 3- inch wafer. This is due to increased depth,
Etch Rate (um/min)
that reduces the effectiveness of supplying reactive
species and removing etch by products. Therefore the
average etch rate achieved for 100 µm etch depths is
much higher than 200 µm etch depths for same diameter 3.5
holes. As reported by other groups, we have also achieved
an etch rate of > 6 µm/min for 100 µm depths using ICP 3
process. However, the reduction in average etch rate with 10 20 30 40 50
etch time is much less for the ICP process in comparison Process Pressure (mTorr)
to the RIE process and etch depths of 176 µm could be
Fig. 4. Etch rate as a function of process Pressure.
achieved in just 45 minutes at 30 mTorr with controlled
(Coil Power=950W, Platen Power=80W, Etch Time=45 Min.)
undercut as shown in Fig. 3. Whereas in case of RIE etch
rate reduced to ~ 1.6 µm/min even at 50 mTorr pressure
the RIE etch profile with higher etch rates. It is evident
and etch depth of 95 µm could only be achieved in 60
from graph that the etch rate is a strong function of
minutes of etching using photoresist mask .
process pressure and is increasing with pressure due to
Fig. 4 shows the ICP process etch rate variation with
increased density of reactive species but anisotropy is
process pressure at 950 W coil power and 80 W platen
maintained mainly due to very small reduction in the ion
power for an etch time of 45 minutes. We have worked
energy incident on the substrate with 10 mTorr increase
around 20-40 mTorr pressure as our aim was to reproduce
in pressure. In other words, physical component of
etching is fairly constant over this narrow pressure range.
Etch rate is increased to 4.4 µm/min at 40 mTorr from
3.7 µm/min at 30 mTorr, for an etch time of 45 minutes,
6 suggesting that the process is at a reaction rate limited
regime in this narrow process pressure window. Fig. 5
shows the SEM cross-section of via hole etched with 4.4
µm/min etch rate. Fig 6 shows etch rate variation as a
0 function of platen power. Increasing platen power to 90
0 10 20 30 40 50 W at pressure 30 mTorr has resulted in reduction in etch
Tim e(Minutes) rate to 3.6 µm/min from 3.9 µm/min at 65 W platen
power for an etch time of 45 minutes contrary to normal
Fig. 2. ICP etch rate variation with elapsed etch time. etch rate variation with platen power at lower pressure
(Coil/Platen Power=950 W / 65 W, Pressure=30 mTorr) range. R. J. Shul et al. have also reported similar trend
JOURNAL OF SEMICONDUCTOR TECHNOLOGY AND SCIENCE, VOL.8, NO.3, SEPTEMBER, 2008 247
Fig. 7. ICP etched via profile at 40mTorr.
Fig. 5. SEM cross-section of via-hole etched with 4.4µm/min
(Coil Power=950W, Platen Power=90W, Etch Time=50 Min.)
etch rate. (Coil Power=950W, Platen Power=80W, Etch
full wafer. This ICP etch profile is almost similar to the
RIE profile (Fig. 1) and is obtained at relatively very
4 high etch rate of ~ 4 µm/min over a 3- inch wafer with
uniformity and reproducibility better than 4%. The etch
selectivity obtained with photoresist mask for this
3.6 process was > 12 : 1.The etched holes were then seed
3.5 metallized and gold plated to form via ground
50 60 70 80 90 100 connections. Fig. 8 shows the SEM photomicrograph of
Platen Pow er(W) gold plated hole from backside with good metal step
coverage. The typical dc via-hole resistance measured
Fig. 6. Etch rate as a function of Platen power. was ~ 0.5 Ω and via inductance value measured was ~
(Coil Power=950W, Pressure =30mTorr, Etch Time=45 Min.) 83 pH for ICP process, well within acceptable range. The
typical dc via resistance and via inductance value
with ICP process in the past . This is probably due to
measured for RIE process were ~ 0.5 Ω and 76 pH
increase in physical etching component and decrease in
respectively. The slightly higher via inductance valve
chemical etching component in comparatively higher
obtained for ICP process is mainly due to marginally
pressure range at 90 W i.e. etching process is more
better an-isotropy over 200 μm depth. Table. 1 shows the
physically driven at 90 W. This reduction in etch rate has
comparison of process parameters for the ICP and RIE
in turn resulted into better etch sidewall morphology at
90 W, because of the higher ion bombardment that may
sputter the surface evenly regardless of defects .
After a series of experiments it was concluded that a
process pressure of 40 mTorr with platen power of 90 W
are suitable for 200 µm deep, 60 µm diameter via-hole
etching. This is due to the fact that etching process using
these values has resulted in high etch rate with similar
etched sidewall morphology as compared to the RIE
process. This indicates that the ICP process would give
better sidewall morphology in comparison to the RIE
process at similar etch rates. Fig. 7 shows the final etch
profile obtained with the ICP process at 40 mTorr
pressure, 950 W coil power, 90 W of platen power for an Fig. 8. SEM photomicrograph of gold plated via-hole from
etch time of 50 min., with via etch yield of > 90% on a backside.
248 D. S. RAWAL et al : A REPRODUCIBLE HIGH ETCH RATE ICP PROCESS FOR ETCHING OF VIA-HOLE GROUNDS IN…
Table 1. RIE/ICP optimized process parameters for 60 μm Authors are also thankful to Shri P. K. Basu, Director,
diameter, 200 μm deep via-hole etching over a 3- inch wafer. SSPL, Delhi for his guidance and giving permission to
S. No. Parameter RIE ICP publish this work.
1. Mask Nickel (2000A°) Photoresist (24μm)
2. Gases CCl2F2/CCl4 Cl2/BCl3 REFERENCES
3. Process Pressure 40mTorr 40mTorr
4. Power 200W 950W/90W
5. Etch Rate ~1.3μm/min. ~ 4μm/min.
 R. E. Williams, GaAs Processing Technology, First
6. Selectivity >200:1 >12:1 edition, p.341, Arctech House, Boston, 1985.
7. Etch Time 180 min. 50 min.  R. A. Pucel, IEEE Trans., MTT-29, 513, 1981.
 L. A. D’ Asaro, J. L. Dilorenzo, and H. Fukui,
process for etching 200 μm deep via holes on 3- inch IEEE Trans., ED-25, 5218, 1978.
wafer with > 90% via yield. The total etch time has been  D. Bonneau, P. Borkowski, R. Shelley, A. Fortier,
significantly reduced from 180 minutes to 50 minutes for M. C. Young, C. Fragos, and S. Anderson, GaAs
ICP etching, with much simpler process using photo- MANTECH Technical Digest, 113, 2002.
resist mask. Finally, this high-density plasma etching  F. Clayton, R Westerman, and D. Johnson, GaAs
process has been integrated in the production line and C- MANTECH Technical Digest, 121, 2002.
band medium power amplifiers/attenuators were fabric-  Vanita. R. Agarwal, D. S. Rawal, and H. P. Vyas, J.
cated with high etch rate, without changing existing MMIC Electrochem. Soc., 152, G567, 2005.
designs and mask sets. These amplifiers and attenuators  R. Westerman, D. Johnson, and M. Devre, Chip
have performed as per the desired specifications, valida- Magazine, 7, 29, 2002.
ting the suitability of the ICP process.  Chih Chang Wang, Yu-Lu Lin, Shun-Kuan Lin,
Chun-Sheng Li, Hou-Kuei Huang, Chang-Luen Wu,
IV. CONCLUSIONS Chian-Sern Chang, and Yeong-Her Wang, J. Vac.
Sci. Technol., B 25(2), 312, 2007.
A 200 μm deep via-hole ICP etching process has been  D. S. Rawal, V. R. Agarwal, H. S. Sharma, B. K.
successfully developed, to replace the existing slow etch Sehgal, R. Gulati, and H. P. Vyas, J. Electrochem.
rate RIE process on 3- inch GaAs wafers, using Cl2/BCl3 Soc., 150, G395, 2003.
gases for the in-house MMIC production line. Desired  Y. W. Chen, B. S. Doi, G. I. Ng, K. Radhakrishnan,
an-isotropic etch profile for 60 μm diameter via-hole and C. L. Tan, J. Vac. Sci. Technol., B 18(5), 2509,
was obtained at 40 mTorr pressure, 950 W coil power, 2000.
90 W of platen power at an etch rate of ~ 4 μm/min and  R. J. Shul, A. G. Baca, R. D. Briggs, G. B. McClellan,
via etch yield of > 90% over a full wafer, with very good S. J. Pearton, and C. Constantine, Sandia National
uniformity and reproducibility. The ICP process has Labs, Albuquerque, NM, Report No. SAND-96-
resulted in high etch rate with acceptable etched sidewall 1901C, 01 Sept 1996.
morphology as compared to the RIE process. Finally,  P. S. Nam, L. M. Ferreira, T. Y. Lee, and K. N. Tu,
this high-density plasma etching process has been inte- J. Vac. Sci. Technol. B, 18, 2780, 2000.
grated in production line for fabrication of MMIC’s with
high throughput, without affecting the production using
existing designs and mask sets.
Authors are thankful to all the members of MMIC
team, Solid State Physics Laboratory, Delhi, India for their
constant support in carrying out the experimental work.
JOURNAL OF SEMICONDUCTOR TECHNOLOGY AND SCIENCE, VOL.8, NO.3, SEPTEMBER, 2008 249
D. S. Rawal received M. Sc. in H. S. Sharma received his M.Sc. in
Physics and M. Tech. in Electronics Physics from Delhi University, India
and Communication Engineering in in 1977. He joined Solid State Physics
1988 and 1990 respectively from Laboratory, Delhi, India in 1978 and
University of Roorkee, India (Now worked for development of GaAs
IIT Roorkee). He is working in the discrete devices, MESFETs and p-
area of GaAs based MMIC Technology since last 15 years HEMTs and their transfer of tech-
and is a recipient of Young Scientist Award and DRDO nology for production. Presently he is a Senior Scientist
Path Breaking Research Award for development of at Solid State Physics Laboratory, Delhi and working for
MMIC technology. Presently he is working as a research the development of p-HEMT based MMIC technology.
scientist in Solid State Physics Laboratory, Delhi for the He has about 20 research papers to his credit. He is a
development of p-HEMT based MMIC Technology. He recipient of DRDO Path Breaking Research Award for
has published more than 35 research papers in various development of 12 GHz MMIC technologies. His present
international journals and conferences. His current research interests include development on GaN HEMT
research interest include dry etch processing of III-V / devices for power applications.
III-N semiconductors and process technology develop-
ment for GaN HEMTs.
B. K. Sehgal is a senior scientist at
the Solid State Physics Laboratory,
Vanita R. Agarwal received M. Sc. Delhi, India. He received M. Tech`
in Chemistry and M. Tech. in Polymer in 1988 from IIT Delhi, India and Ph.
Science and Technology from IIT D. in 2003 from University of Delhi,
Delhi, India in 1984 and 1986 res- Delhi, India. He has more than 25
pectively. She was Senior Scientific years of experience in the develop-
Officer at IIT Delhi from 1986 to ment of GaAs microwave device technology. Currently,
1988. She joined Solid State Physics he is leading a group of scientists working on the
Laboratory, Delhi in 1988 and worked on growth of III- development of MESFET’s, HEMT’s and MMIC’s and
V compounds. Presently she is working as a research their technology transfer for production. He has
scientist at Solid State Physics Laboratory, Delhi for the published more than 20 research papers and is a recipient
development of Fabrication Technology related to GaAs of Young Scientist Award and DRDO Path Breaking
based MMICs. She has published 18 research papers in Research Award for development of 12 GHz MMIC
various international journals and conferences and is a technologies.
recipient of DRDO Outstanding Team Work Award for
development of MMIC technology. Her current research
interest include dry etch processing of semiconductors,
Flip Chip Technology for III-V based MMICs and
processing of GaN based MMICs.
250 D. S. RAWAL et al : A REPRODUCIBLE HIGH ETCH RATE ICP PROCESS FOR ETCHING OF VIA-HOLE GROUNDS IN…
R. Muralidharan is presently
Director of Solid State Physics
Laboratory, Delhi, India and CEO of
GAETEC, Hyderabad, India. He
obtained his M.Sc. in Physics in
1975 from Madras and Ph.D. in 1985
from IISc, Bangalore. His main areas of work include
MBE growth & characterization of epitaxial layers for
high electron mobility transistors, quantum dot devices
and production of MMIC modules for micro-wave
applications. He has a valuable research experience of
more than 25 years in the field of III-V compounds. He
has published more than 30 research papers in various
international journals and conferences and is the
recipient of MRSI Medal- 1989, Science Day Award-
2003 and Technology Group Award for Advancement in
Material Growth Technology using MBE.